Article Cite This: Ind. Eng. Chem. Res. XXXX, XXX, XXX−XXX
Mechanisms of Copper-Based Catalyst Deactivation during CO2 Reduction to Methanol Anže Prašnikar,*,† Andraž Pavlišic,̌ † Francisco Ruiz-Zepeda,∥ Janez Kovac,̌ § and Blaž Likozar*,† †
Downloaded via BUFFALO STATE on July 19, 2019 at 03:12:47 (UTC). See https://pubs.acs.org/sharingguidelines for options on how to legitimately share published articles.
Department of Catalysis and Chemical Reaction Engineering, National Institute of Chemistry, Hajdrihova 19, 1000 Ljubljana, Slovenia ∥ Department of Materials Chemistry, National Institute of Chemistry, Hajdrihova 19, 1000 Ljubljana, Slovenia § Department of Surface Engineering and Optoelectronics, Jožef Stefan Institute, Jamova 39, 1000 Ljubljana, Slovenia S Supporting Information *
ABSTRACT: Despite the fact that the methanol synthesis process includes industrially some of the most important catalytic chemical reactions, it is still not clear how diﬀerent gaseous species impact catalyst component structure. With the goal to reduce CO2 emissions through hydrogenation to CH3OH, a higher H2O formation rate than in the production from compressed CO-rich feed should also be considered. It is known that steam accelerates the sintering of metals, several oxide compounds, and their interfaces. To determine the eﬀect of moisture on the Cu/ZnO/Al2O3 catalysts, a commercial catalytic material was systematically aged at various gas compositions and analyzed using transient H2 surface adsorption, N2O pulse eﬃcient chemisorption, X-ray photoelectron spectroscopy, scanning transmission electron microscopy mapping, X-ray powder diﬀraction, and N2 physisorption, and the mechanisms of deactivation were observed. A strong consistent relation between the compacting of Al2O3, the amount of water in the controlled streamﬂow, and the activity was found. This connected loss of support resulted in the (re)forming of Cu, ZnO, and Cu/ZnO phases. Copper particle growth was modeled by applying a physical coalescence model. In the presence of CO and/or CH3OH, zinc oxide material started to cover the Cu granules, while H2O promoted the development of separate Cu regions.
1. INTRODUCTION Methanol is an important chemical for the production of various products such as dimethyl ether, formaldehyde, and acetic acid. Besides being a feedstock chemical, methanol can also be mixed with gasoline and used as a mixture.1 It can be produced to capture CO2 emissions from carbon-rich sources such as steel plants and thermoelectric power stations. Conventionally, methanol is synthesized using syn-gas in a packed bed reactor with a recycle at 240−280 °C and 50−100 bar with Cu/ZnO/Al2O3 (CZA) catalyst. The CZA catalysts are usually used for several years with gradual temperature increase in the reactor to compensate for the activity decrease.2 Catalysts can be deactivated by particle sintering or sulfur and halogenide poisoning.3,4 Poisoning is usually eliminated by sulfur/halogenide removal processes;5,6 however, sintering cannot be simply omitted. The rate of deactivation is usually limited by the addition of refractory © XXXX American Chemical Society
materials (Al2O3, SiO2, MgO, etc.), which act as a support for active components.7−9 In addition to the thermal sintering, gas atmosphere can accelerate this process by increasing surface diﬀusion of the catalyst molecules.10−12 The surface diﬀusion of hydroxylated ZnO is faster than that for pure ZnO, resulting in a higher sintering rate.12 The rate of bulk diﬀusion is also dependent on the gaseous environment. For example, Gai et al.13 observed increased diﬀusion of copper through the alumina layer in the presence of oxygen, which they correlated with surface energy minimization. Recently it was shown, that ZnO grows over Cu particles under the reaction conditions implemented during Received: Revised: Accepted: Published: A
April 8, 2019 June 28, 2019 June 29, 2019 July 1, 2019 DOI: 10.1021/acs.iecr.9b01898 Ind. Eng. Chem. Res. XXXX, XXX, XXX−XXX
Industrial & Engineering Chemistry Research methanol synthesis, resulting in decreased copper surface area.14,15 The catalysts for the methanol synthesis were optimized for the conversion of CO-rich syn-gas, however, the deactivation process could proceed diﬀerently in the case of pure CO2 reduction by H2. This would be due to larger H2O and smaller CO content, since for every molecule of CO2 an additional molecule of H2O is formed. It is widely known that steam increases the sintering rate of oxides and metal particles and therefore decreases active surface area.9,11,12,16−21 Steam impacts the catalyst activity temporarily (reversibly) and permanently (irreversibly). Some existing literature has been presented on reversible catalyst deactivation by H2O,22−24 which is caused by occupation of the active sites with *OH.24 The rate of methanol formation increases in the presence of CO, which scavenge surface hydroxyls through the water gas shift reaction (WGS). The irreversible deactivation was also studied for Cu/ZnO/ZrO/Al2O3 catalysts with steam being added into the stream,9,16 indicating that H2O increased the rate of deactivation. The rate of deactivation was reduced by the addition of colloid silica, which additionally stabilized the catalyst structure.9 However, there was no detailed post-mortem catalyst characterization to determine the deactivation mechanism with H2O or determination of catalyst morphology changes. For this reason, we performed experiments with the CZA catalyst under diﬀerent aging compositions at 50 bar and 240 °C for 48 h with the purpose of isolating the eﬀect of H2O. The samples after and before aging were analyzed with various techniques to provide a clear picture of structural changes of catalyst samples. The model of H2O eﬀect on Cu particle growth is presented. The changes of the catalytic activity were explained by structural transformations.
Figure 1. Experimental work procedure.
equipped with CP-Molsieve and PoraPlot U columns.). A preprepared gas mixture of H2/CO2/N2 = 61/29/10 (TPJ, d.o.o., Jesenice) and pure H2 with purities 99.999% (Messer) were mixed to obtain gas inlet mixtures. In the case of samples R1 and R5, distilled water was pumped with a HPLC pump into the vaporizer where it was mixed with the other gases. The aging conditions and inlet compositions are displayed in Table 1. Table 1. Catalyst Aging Conditions (Temperature, 240 °C; Pressure, 50 bar) name
inlet aging gas composition H2/CO2/H2O/N2
R1 R2 R3 R4 R5 R6 R7 R8
62/24.8/5.6/7.6 65/26/0/8 65/26/0/8 65/26/0/8 93.1/0/6.9/0 only reduction 100/0/0/0 no aging
40 000 20 000 1 700 40 000 40 000 13 000
The X-ray photoelectron spectroscopy (XPS) analyses were carried out on the PHI-TFA XPS spectrometer produced by Physical Electronics Inc. Sample powders were brought from the catalytic reactor under the protective atmosphere of Ar and introduced into an ultra-high-vacuum spectrometer. The analyzed area was 0.4 mm in diameter and the analyzed depth was about 3−5 nm. Sample surfaces were excited by Xray radiation from a monochromatic Al source at a photon energy of 1486.6 eV. The high-energy resolution spectra were acquired with a pass energy of 29 eV and an energy resolution of 0.6 eV. Because of the favorable electrical conductivity of the graphite phase involved in the samples, XPS spectra were not aligned since no charging eﬀects were observed. The accuracy of binding energies was about ±0.3 eV. Quantiﬁcation of surface composition was performed from XPS peak intensities taking into account relative sensitivity factors provided by the instrument manufacturer. Two diﬀerent XPS measurements were performed on each sample and the average composition was calculated. Samples for the XRD analyses were powdered and transferred in the inert atmosphere on the XRD holder and covered with the Kapton ﬁlm. The analyses were performed on the PANalytical X’Pert Pro instrument. The CuKα1 radiation source was used for the scanning from 10° to 90°. Afterward, Rietveld reﬁnement of the XRD patterns was performed to extract the crystal size and phase composition using the Fm3m, P63mc, and Fd3m of Cu, ZnO, and Al2ZnO4 spinel, respectively. The instrumental resolution function was determined by reﬁnement of the XRD pattern of a SiO2 standard powder. For the ﬁtting procedure, X’Pert HighScore Plus was used with U and W coeﬃcients for description of
2. EXPERIMENTAL SECTION To determine the eﬀect of the H2O on the methanol catalyst, approximately 400 mg of pelletized commercial Cu/ZnO/ Al2O3 catalyst HiFuel W230 (particle sizes 200−400 μm) was inserted into the parallel packed bed reactor system and aged under diﬀerent conditions. Aging was performed in the same reactor as was used for the catalytic tests. The scheme of parallel packed bed reactor system and ﬁlled reactor tube can be found in the Supporting Information, section S6. The catalyst contains 50.2 wt % of CuO, 30.8 wt % of ZnO, and 18.7 wt % of Al2O3 with the addition of graphite as a binder. Before being aged, the samples were reduced in H2 at 1 bar and 300 °C for 12 h and evaluated in H2/CO2 = 2.5 at 50 bar, 180−240 °C and GHSV 40 000 h−1 (long form NmLgas mLcat−1 h−1). Catalytic activity was measured again after aging (shown only for 240 °C). In both catalytic tests, catalysts were held at 240 °C for 8 h to ensure that the change in catalyst activity is solely due to the irreversible catalyst changes, for example, alterations due to irreversible catalyst morphology and not from adsorbed species remaining following aging. The samples were transferred and prepared in a glovebox (for the X-ray photoelectron spectroscopy (XPS) and X-ray diﬀraction (XRD) analyses) or were passivated using N2O (for the scanning transmission electron microscopy (STEM), N 2 physisorption, and chemisorption analyses). Figure 1 shows experimental procedure. Catalytic tests and aging were performed in a parallel reactor system with online gas composition analysis using gas chromatography (Agilent 490 Micro GC, TCD detectors B
DOI: 10.1021/acs.iecr.9b01898 Ind. Eng. Chem. Res. XXXX, XXX, XXX−XXX
Industrial & Engineering Chemistry Research
Figure 2. Particle sizes of Cu (red) and ZnO (blue) determined using XRD by Rietveld reﬁnement. CO2 conversion (green) is measured after aging at 240 °C, 50 bar, GHSV of 40 000 h−1.
Table 2. Average Volume Gas Compositions of Aging Gas Mixtures average aging volume fraction [%] name R1 R2 R3 R4 R6 R7 R8 R9
H2/CO2 low conv. + 6%H2O H2/CO2 med. conv. H2/CO2 eq. conv. H2/CO2 low conv. H2 + 6% H2O only reduction H2 no aging
61.9 63.4 59.1 64 93.1
23.8 23.2 20 24
6.1 2.4 6 1.9 6.9
0.3 0.9 1.6 0.6
0.1 1.1 4.5 1
7.8 9 8.8 8.5
3. RESULTS AND DISCUSSION The Cu and ZnO particle sizes and CO2 conversion after diﬀerent treatments are displayed in Figure 2. Average particle sizes were determined with XRD using Rietveld reﬁnement, while the CO2 conversions were obtained from the second catalytic tests. Since samples were tested in the parallel reactor system, there are minor diﬀerences (